Page:EB1911 - Volume 07.djvu/123

Rh material liberates the metallic copper. The metal is so pure that it can be refined by a continuous operation in the same furnace.

Wet Methods for Copper Extraction.—Wet methods are only employed for low grade ores (under favourable circumstances ore containing from ¼ to 1% of copper has admitted of economic treatment), and for gold and silver bearing metallurgical products.

The fundamental principle consists in getting the ore into a solution, from which the metal can be precipitated. The ores of any economic importance contain the copper either as oxide, carbonate, sulphate or sulphide. These compounds are got into solution either as chlorides or sulphates, and from either of these salts the metal can be readily obtained. Ores in which the copper is present as oxide or carbonate are soluble in sulphuric or hydrochloric acids, ferrous chloride, ferric sulphate, ammoniacal compounds and sodium thiosulphate. Of these solvents, only the first three are of economic importance. The choice of sulphuric or hydrochloric acid depends mainly upon the cost, both acting with about the same rapidity; thus if a Leblanc soda factory is near at hand, then hydrochloric acid would most certainly be employed. Ferrous chloride is not much used; the Douglas-Hunt process uses a mixture of salt and ferrous sulphate which involves the formation of ferrous chloride, and the new Douglas-Hunt process employs sulphuric acid in which ferrous chloride is added after leaching.

Sulphuric acid may be applied as such on the ores placed in lead, brick, or stone chambers; or as a mixture of sulphur dioxide, nitrous fumes (generated from Chile saltpetre and sulphuric acid), and steam, which permeates the ore resting on the false bottom of a brick chamber. When most of the copper has been converted into the sulphate, the ore is lixiviated. Hydrochloric acid is applied in the same way as sulphuric acid; it has certain advantages of which the most important is that it does not admit the formation of basic salts; its chief disadvantage is that it dissolves the oxides of iron, and accordingly must not be used for highly ferriferous ores. The solubility of copper carbonate in ferrous chloride solution was pointed out by Max Schaffner in 1862, and the subsequent recognition of the solubility of the oxide in the same solvent by James Douglas and Sterry Hunt resulted in the “Douglas-Hunt” process for the wet extraction of copper. Ferrous chloride decomposes the copper oxide and carbonate with the formation of cuprous and cupric chlorides (which remain in solution), and the precipitation of ferrous oxide, carbon dioxide being simultaneously liberated from the carbonate. In the original form of the Douglas-Hunt process, ferrous chloride was formed by the interaction of sodium chloride (common salt) with ferrous sulphate (green vitriol), the sodium sulphate formed at the same time being removed by crystallization. The ground ore was stirred with this solution at 70° C. in wooden tubs until all the copper was dissolved. The liquor was then filtered from the iron oxides, and the filtrate treated with scrap iron, which precipitated the copper and reformed ferrous chloride, which could be used in the first stage of the process. The advantage of this method rests chiefly on the small amount of iron required; but its disadvantages are that any silver present in the ores goes into solution, the formation of basic salts, and the difficulty of filtering from the iron oxides. A modification of the method was designed to remedy these defects. The ore is first treated with dilute sulphuric acid, and then ferrous or calcium chloride added, thus forming copper chlorides. If calcium chloride be used the precipitated calcium sulphate must be removed by filtration. Sulphur dioxide is then blown in, and the precipitate is treated with iron, which produces metallic copper, or milk of lime, which produces cuprous oxide. Hot air is blown into the filtrate, which contains ferrous or calcium chlorides, to expel the excess of sulphur dioxide, and the liquid can then be used again. In this process (“new Douglas-Hunt”) there are no iron oxides formed, the silver is not dissolved, and the quantity of iron necessary is relatively small, since all the copper is in the cuprous condition. It is not used in the treatment of ores, but finds application in the case of calcined argentiferous lead and copper mattes.

The precipitation of the copper from the solution, in which it is present as sulphate, or as cuprous and cupric chlorides, is generally effected by metallic iron. Either wrought, pig, iron sponge or iron bars are employed, and it is important to notice that the form in which the copper is precipitated, and also the time taken for the separation, largely depend upon the condition in which the iron is applied. Spongy iron acts most rapidly, and after this follow iron turnings and then sheet clippings. Other precipitants such as sulphuretted hydrogen and solutions of sulphides, which precipitate the copper as sulphides, and milk of lime, which gives copper oxides, have not met with commercial success. When using iron as the precipitant, it is desirable that the solution should be as neutral as possible, and the quantity of ferric salts present should be reduced to a minimum; otherwise, a certain amount of iron would be used up by the free acid and in reducing the ferric salts. Ores in which the copper is present as sulphate are directly lixiviated and treated with iron. Mine waters generally contain the copper in this form, and it is extracted by conducting the waters along troughs fitted with iron gratings.

The wet extraction of metallic copper from ores in which it occurs as the sulphide, may be considered to involve the following operations: (1) conversion of the copper into a soluble form, (2) dissolving out the soluble copper salt, (3) the precipitation of the copper. Copper sulphide may be converted either into the sulphate, which is soluble in water; the oxide, soluble in sulphuric or hydrochloric acid; cupric chloride, soluble in water; or cuprous chloride, which is soluble in solutions of metallic chlorides.

The conversion into sulphate is generally effected by the oxidizing processes of weathering, calcination, heating with iron nitrate or ferric sulphate. It may also be accomplished by calcination with ferrous sulphate, or other easily decomposable sulphates, such as aluminium sulphate. Weathering is a very slow, and, therefore, an expensive process; moreover, the entire conversion is only accomplished after a number of years. Calcination is only advisable for ores which contain relatively much iron pyrites and little copper pyrites. Also, however slowly the calcination may be conducted, there is always more or less copper sulphide left unchanged, and some copper oxide formed. Calcination with ferrous sulphate converts all the copper sulphide into sulphate. Heap roasting has been successfully employed at Agordo, in the Venetian Alps, and at Majdanpek in Servia. Josef Perino’s process, which consists in heating the ore with iron nitrate to 50°–150° C., is said to possess several advantages, but it has not been applied commercially. Ferric sulphate is only used as an auxiliary to the weathering process and in an electrolytic process.

The conversion of the sulphide into oxide is adopted where the Douglas-Hunt process is employed, or where hydrochloric or sulphuric acids are cheap. The calcination is effected in reverberatory furnaces, or in muffle furnaces, if the sulphur is to be recovered. Heap, stall or shaft furnace roasting is not very satisfactory, as it is very difficult to transform all the sulphide into oxide.

The conversion of copper sulphide into the chlorides may be accomplished by calcining with common salt, or by treating the ores with ferrous chloride and hydrochloric acid or with ferric chloride. The dry way is best; the wet way is only employed when fuel is very dear, or when it is absolutely necessary that no noxious vapours should escape into the atmosphere. The dry method consists in an oxidizing roasting of the ores, and a subsequent chloridizing roasting with either common salt or Abraumsalz in reverberatory or muffle furnaces. The bulk of the copper is thus transformed into cupric chloride, little cuprous chloride being obtained. This method had been long proposed by William Longmaid, Max Schaffner, Becchi and Haupt, but was only introduced into England by the labours of William Henderson, J. A. Phillips and others. The wet method is employed at Rio Tinto, the particular variant being known as the “Dötsch” process. This consists in stacking the broken ore in heaps and adding a mixture of sodium sulphate and ferric